#------------------------------------------------------------------------------
#$Date: 2016-02-20 00:18:51 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176760 $
#$URL: svn://www.crystallography.net/cod/cif/2/01/52/2015288.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2015288
loop_
_publ_author_name
'Demchenko, Pavlo'
'Kończyk, Joanna'
'Demchenko, Grigorii'
'Gladyshevskii, Roman'
'Pavlyuk, Volodymyr'
_publ_section_title
;
 Er₅Ni₃Al₃Ge₄: a quaternary variant of the NbCoB type
;
_journal_coeditor_code           BC1097
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              i29
_journal_page_last               i31
_journal_paper_doi               10.1107/S0108270106009255
_journal_volume                  62
_journal_year                    2006
_chemical_formula_iupac          'Er5 Ni3 Al3 Ge4'
_chemical_formula_moiety         'Al3 Er5 Ge4 Ni3'
_chemical_formula_sum            'Al3 Er5 Ge4 Ni3'
_chemical_formula_weight         1383.73
_chemical_name_common
'Pentaerbium trinickel trialuminum tetragermanide'
_chemical_name_systematic
;
pentaerbium trinickel trialuminium tetragermanium
;
_space_group_IT_number           59
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ab 2a'
_symmetry_space_group_name_H-M   'P m m n :2'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   4.1561(6)
_cell_length_b                   19.0690(10)
_cell_length_c                   6.8369(5)
_cell_measurement_reflns_used    18
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      33
_cell_measurement_theta_min      15
_cell_volume                     541.84(9)
_computing_cell_refinement       'KM4B8 Software'
_computing_data_collection
'KM4B8 Software (Galdecki et al.,  1996)'
_computing_data_reduction        'KM4B8 Software'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Kuma KM-4'
_diffrn_measurement_method       ω-2θ
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0849
_diffrn_reflns_av_sigmaI/netI    0.0327
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            3581
_diffrn_reflns_theta_full        68.01
_diffrn_reflns_theta_max         68.01
_diffrn_reflns_theta_min         4.64
_diffrn_standards_decay_%        2
_diffrn_standards_interval_count 100
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    87.553
_exptl_absorpt_correction_T_max  0.3817
_exptl_absorpt_correction_T_min  0.1688
_exptl_absorpt_correction_type   cylinder
_exptl_absorpt_process_details   '(Dwiggins, 1975)'
_exptl_crystal_colour            'metallic dark grey'
_exptl_crystal_density_diffrn    8.481
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'elongated prism'
_exptl_crystal_F_000             1182
_exptl_crystal_size_max          0.11
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.011
_refine_diff_density_max         3.990
_refine_diff_density_min         -2.751
_refine_ls_extinction_coef       0.00070(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL97
_refine_ls_goodness_of_fit_ref   1.164
_refine_ls_matrix_type           full
_refine_ls_number_parameters     50
_refine_ls_number_reflns         580
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.164
_refine_ls_R_factor_all          0.0492
_refine_ls_R_factor_gt           0.0431
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0783P)²+0.734P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1079
_refine_ls_wR_factor_ref         0.1106
_reflns_number_gt                501
_reflns_number_total             580
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            bc1097.cif
_cod_data_source_block           I
_cod_original_sg_symbol_H-M      'P m m n'
_cod_database_code               2015288
_cod_database_fobs_code          2015288
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y+1/2, z'
'x+1/2, -y, -z'
'-x, y+1/2, -z'
'-x, -y, -z'
'x-1/2, y-1/2, -z'
'-x-1/2, y, z'
'x, -y-1/2, z'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
Er Er1 0.2500 0.57155(5) 0.49989(10) 0.0180(4) Uani d S 1
Er Er2 0.2500 0.61950(5) 0.99676(11) 0.0175(4) Uani d S 1
Er Er3 0.2500 0.7500 0.61585(17) 0.0178(4) Uani d S 1
Ge Ge1 0.2500 0.03874(9) 0.7965(2) 0.0177(5) Uani d S 1
Ge Ge2 0.2500 0.14615(8) 0.2890(2) 0.0172(5) Uani d S 1
Ni Ni1 0.2500 0.02588(14) 0.1663(4) 0.0199(6) Uani d S 1
Ni Ni2 0.2500 0.7500 0.2066(5) 0.0217(9) Uani d S 1
Al Al1 0.2500 0.1784(2) 0.6850(6) 0.0134(9) Uani d S 1
Al Al2 0.2500 0.2500 0.0285(8) 0.0137(13) Uani d S 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.2130 0.2455 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -9.4367 3.9380 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge -1.0885 0.8855 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni -3.0029 0.5091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
Ge2 Er1 Ge2 6_666 6_566 91.43(5)
Ge2 Er1 Ge1 6_666 2 90.44(4)
Ge2 Er1 Ge1 6_566 2 90.44(4)
Ge2 Er1 Ni1 6_666 2 134.03(3)
Ge2 Er1 Ni1 6_566 2 134.03(3)
Ge1 Er1 Ni1 2 2 94.79(7)
Ge2 Er1 Ge1 6_666 6_566 160.68(5)
Ge2 Er1 Ge1 6_566 6_566 86.65(3)
Ge1 Er1 Ge1 2 6_566 108.78(4)
Ni1 Er1 Ge1 2 6_566 48.53(4)
Ge2 Er1 Ge1 6_666 6_666 86.65(3)
Ge2 Er1 Ge1 6_566 6_666 160.68(5)
Ge1 Er1 Ge1 2 6_666 108.78(4)
Ni1 Er1 Ge1 2 6_666 48.53(4)
Ge1 Er1 Ge1 6_566 6_666 88.84(5)
Ge2 Er1 Al1 6_666 6_666 54.16(7)
Ge2 Er1 Al1 6_566 6_666 110.61(7)
Ge1 Er1 Al1 2 6_666 137.63(5)
Ni1 Er1 Al1 2 6_666 95.56(8)
Ge1 Er1 Al1 6_566 6_666 108.77(7)
Ge1 Er1 Al1 6_666 6_666 53.50(7)
Ge2 Er1 Al1 6_666 6_566 110.61(7)
Ge2 Er1 Al1 6_566 6_566 54.16(7)
Ge1 Er1 Al1 2 6_566 137.63(5)
Ni1 Er1 Al1 2 6_566 95.56(8)
Ge1 Er1 Al1 6_566 6_566 53.50(7)
Ge1 Er1 Al1 6_666 6_566 108.77(7)
Al1 Er1 Al1 6_666 6_566 81.81(10)
Ge2 Er1 Ni1 6_666 6_666 46.79(5)
Ge2 Er1 Ni1 6_566 6_666 104.06(5)
Ge1 Er1 Ni1 2 6_666 46.41(4)
Ni1 Er1 Ni1 2 6_666 112.35(5)
Ge1 Er1 Ni1 6_566 6_666 151.88(7)
Ge1 Er1 Ni1 6_666 6_666 88.57(4)
Al1 Er1 Ni1 6_666 6_666 91.93(6)
Al1 Er1 Ni1 6_566 6_666 151.90(9)
Ge2 Er1 Ni1 6_666 6_566 104.06(5)
Ge2 Er1 Ni1 6_566 6_566 46.79(5)
Ge1 Er1 Ni1 2 6_566 46.41(4)
Ni1 Er1 Ni1 2 6_566 112.35(5)
Ge1 Er1 Ni1 6_566 6_566 88.57(4)
Ge1 Er1 Ni1 6_666 6_566 151.88(7)
Al1 Er1 Ni1 6_666 6_566 151.90(9)
Al1 Er1 Ni1 6_566 6_566 91.93(6)
Ni1 Er1 Ni1 6_666 6_566 80.77(6)
Ge2 Er1 Er1 6_666 5_566 145.43(5)
Ge2 Er1 Er1 6_566 5_566 87.47(3)
Ge1 Er1 Er1 2 5_566 55.04(3)
Ni1 Er1 Er1 2 5_566 59.86(4)
Ge1 Er1 Er1 6_566 5_566 53.75(3)
Ge1 Er1 Er1 6_666 5_566 104.88(5)
Al1 Er1 Er1 6_666 5_566 155.22(8)
Al1 Er1 Er1 6_566 5_566 96.57(5)
Ni1 Er1 Er1 6_666 5_566 100.15(5)
Ni1 Er1 Er1 6_566 5_566 52.49(5)
Ge2 Er1 Er1 6_666 5_666 87.47(3)
Ge2 Er1 Er1 6_566 5_666 145.43(5)
Ge1 Er1 Er1 2 5_666 55.04(3)
Ni1 Er1 Er1 2 5_666 59.86(4)
Ge1 Er1 Er1 6_566 5_666 104.88(5)
Ge1 Er1 Er1 6_666 5_666 53.75(3)
Al1 Er1 Er1 6_666 5_666 96.57(5)
Al1 Er1 Er1 6_566 5_666 155.22(8)
Ni1 Er1 Er1 6_666 5_666 52.49(5)
Ni1 Er1 Er1 6_566 5_666 100.15(5)
Er1 Er1 Er1 5_566 5_666 74.58(4)
Ge2 Er1 Er3 6_666 . 53.83(3)
Ge2 Er1 Er3 6_566 . 53.83(3)
Ge1 Er1 Er3 2 . 122.93(5)
Ni1 Er1 Er3 2 . 142.28(6)
Ge1 Er1 Er3 6_566 . 111.10(4)
Ge1 Er1 Er3 6_666 . 111.10(4)
Al1 Er1 Er3 6_666 . 57.64(7)
Al1 Er1 Er3 6_566 . 57.64(7)
Ni1 Er1 Er3 6_666 . 95.91(6)
Ni1 Er1 Er3 6_566 . 95.91(6)
Er1 Er1 Er3 5_566 . 140.78(2)
Er1 Er1 Er3 5_666 . 140.78(2)
Ge2 Er1 Er2 6_666 . 52.59(3)
Ge2 Er1 Er2 6_566 . 52.59(3)
Ge1 Er1 Er2 2 . 61.11(4)
Ni1 Er1 Er2 2 . 155.90(6)
Ge1 Er1 Er2 6_566 . 135.54(3)
Ge1 Er1 Er2 6_666 . 135.54(3)
Al1 Er1 Er2 6_666 . 102.57(7)
Al1 Er1 Er2 6_566 . 102.57(7)
Ni1 Er1 Er2 6_666 . 51.93(4)
Ni1 Er1 Er2 6_566 . 51.93(4)
Er1 Er1 Er2 5_566 . 101.91(3)
Er1 Er1 Er2 5_666 . 101.91(3)
Er3 Er1 Er2 . . 61.82(3)
Ge2 Er1 Er2 6_666 1_554 110.77(4)
Ge2 Er1 Er2 6_566 1_554 110.77(4)
Ge1 Er1 Er2 2 1_554 148.84(5)
Ni1 Er1 Er2 2 1_554 54.05(6)
Ge1 Er1 Er2 6_566 1_554 52.74(3)
Ge1 Er1 Er2 6_666 1_554 52.74(3)
Al1 Er1 Er2 6_666 1_554 56.64(6)
Al1 Er1 Er2 6_566 1_554 56.64(6)
Ni1 Er1 Er2 6_666 1_554 139.25(3)
Ni1 Er1 Er2 6_566 1_554 139.25(3)
Er1 Er1 Er2 5_566 1_554 101.82(3)
Er1 Er1 Er2 5_666 1_554 101.82(3)
Er3 Er1 Er2 . 1_554 88.23(3)
Er2 Er1 Er2 . 1_554 150.05(4)
Ni2 Er2 Ge2 1_556 6_566 100.65(6)
Ni2 Er2 Ge2 1_556 6_666 100.65(6)
Ge2 Er2 Ge2 6_566 6_666 91.66(5)
Ni2 Er2 Ge1 1_556 6_567 102.30(6)
Ge2 Er2 Ge1 6_566 6_567 84.80(3)
Ge2 Er2 Ge1 6_666 6_567 157.04(6)
Ni2 Er2 Ge1 1_556 6_667 102.30(6)
Ge2 Er2 Ge1 6_566 6_667 157.04(6)
Ge2 Er2 Ge1 6_666 6_667 84.80(3)
Ge1 Er2 Ge1 6_567 6_667 89.66(5)
Ni2 Er2 Ni1 1_556 6_566 135.33(4)
Ge2 Er2 Ni1 6_566 6_566 49.29(6)
Ge2 Er2 Ni1 6_666 6_566 110.84(6)
Ge1 Er2 Ni1 6_567 6_566 50.95(6)
Ge1 Er2 Ni1 6_667 6_566 111.14(6)
Ni2 Er2 Ni1 1_556 6_666 135.33(4)
Ge2 Er2 Ni1 6_566 6_666 110.84(6)
Ge2 Er2 Ni1 6_666 6_666 49.29(6)
Ge1 Er2 Ni1 6_567 6_666 111.14(6)
Ge1 Er2 Ni1 6_667 6_666 50.95(6)
Ni1 Er2 Ni1 6_566 6_666 89.27(7)
Ni2 Er2 Ni1 1_556 2_556 127.34(9)
Ge2 Er2 Ni1 6_566 2_556 114.96(5)
Ge2 Er2 Ni1 6_666 2_556 114.96(5)
Ge1 Er2 Ni1 6_567 2_556 48.16(3)
Ge1 Er2 Ni1 6_667 2_556 48.16(3)
Ni1 Er2 Ni1 6_566 2_556 65.70(7)
Ni1 Er2 Ni1 6_666 2_556 65.70(7)
Ni2 Er2 Al1 1_556 6_667 50.09(7)
Ge2 Er2 Al1 6_566 6_667 149.26(7)
Ge2 Er2 Al1 6_666 6_667 86.06(6)
Ge1 Er2 Al1 6_567 6_667 108.30(7)
Ge1 Er2 Al1 6_667 6_667 53.26(7)
Ni1 Er2 Al1 6_566 6_667 157.09(9)
Ni1 Er2 Al1 6_666 6_667 90.68(6)
Ni1 Er2 Al1 2_556 6_667 93.53(8)
Ni2 Er2 Al1 1_556 6_567 50.09(7)
Ge2 Er2 Al1 6_566 6_567 86.06(6)
Ge2 Er2 Al1 6_666 6_567 149.26(7)
Ge1 Er2 Al1 6_567 6_567 53.26(7)
Ge1 Er2 Al1 6_667 6_567 108.30(7)
Ni1 Er2 Al1 6_566 6_567 90.68(6)
Ni1 Er2 Al1 6_666 6_567 157.09(9)
Ni1 Er2 Al1 2_556 6_567 93.53(8)
Al1 Er2 Al1 6_667 6_567 80.63(9)
Ni2 Er2 Al2 1_556 5_666 50.40(8)
Ge2 Er2 Al2 6_566 5_666 106.78(8)
Ge2 Er2 Al2 6_666 5_666 50.99(9)
Ge1 Er2 Al2 6_567 5_666 151.31(10)
Ge1 Er2 Al2 6_667 5_666 88.55(6)
Ni1 Er2 Al2 6_566 5_666 153.16(11)
Ni1 Er2 Al2 6_666 5_666 89.59(6)
Ni1 Er2 Al2 2_556 5_666 136.69(6)
Al1 Er2 Al2 6_667 5_666 49.74(12)
Al1 Er2 Al2 6_567 5_666 100.48(9)
Ni2 Er2 Al2 1_556 5_566 50.40(8)
Ge2 Er2 Al2 6_566 5_566 50.99(9)
Ge2 Er2 Al2 6_666 5_566 106.78(8)
Ge1 Er2 Al2 6_567 5_566 88.55(6)
Ge1 Er2 Al2 6_667 5_566 151.31(10)
Ni1 Er2 Al2 6_566 5_566 89.59(6)
Ni1 Er2 Al2 6_666 5_566 153.16(11)
Ni1 Er2 Al2 2_556 5_566 136.69(6)
Al1 Er2 Al2 6_667 5_566 100.48(9)
Al1 Er2 Al2 6_567 5_566 49.74(12)
Al2 Er2 Al2 5_666 5_566 79.59(2)
Ni2 Er2 Ge1 1_556 2 174.44(8)
Ge2 Er2 Ge1 6_566 2 83.17(4)
Ge2 Er2 Ge1 6_666 2 83.17(4)
Ge1 Er2 Ge1 6_567 2 73.88(5)
Ge1 Er2 Ge1 6_667 2 73.89(5)
Ni1 Er2 Ge1 6_566 2 45.14(4)
Ni1 Er2 Ge1 6_666 2 45.14(4)
Ni1 Er2 Ge1 2_556 2 47.09(6)
Al1 Er2 Ge1 6_667 2 126.77(7)
Al1 Er2 Ge1 6_567 2 126.77(7)
Al2 Er2 Ge1 5_666 2 132.53(6)
Al2 Er2 Ge1 5_566 2 132.53(7)
Ni2 Er2 Er1 1_556 . 135.03(7)
Ge2 Er2 Er1 6_566 . 52.73(3)
Ge2 Er2 Er1 6_666 . 52.73(3)
Ge1 Er2 Er1 6_567 . 109.11(4)
Ge1 Er2 Er1 6_667 . 109.11(4)
Ni1 Er2 Er1 6_566 . 58.62(5)
Ni1 Er2 Er1 6_666 . 58.62(5)
Ni1 Er2 Er1 2_556 . 97.62(6)
Al1 Er2 Er1 6_667 . 138.17(5)
Al1 Er2 Er1 6_567 . 138.17(5)
Al2 Er2 Er1 5_666 . 98.50(10)
Al2 Er2 Er1 5_566 . 98.50(10)
Ge1 Er2 Er1 2 . 50.53(3)
Ni2 Er2 Er1 1_556 1_556 74.92(7)
Ge2 Er2 Er1 6_566 1_556 134.17(3)
Ge2 Er2 Er1 6_666 1_556 134.17(3)
Ge1 Er2 Er1 6_567 1_556 53.29(3)
Ge1 Er2 Er1 6_667 1_556 53.29(3)
Ni1 Er2 Er1 6_566 1_556 102.07(6)
Ni1 Er2 Er1 6_666 1_556 102.07(6)
Ni1 Er2 Er1 2_556 1_556 52.43(5)
Al1 Er2 Er1 6_667 1_556 55.61(7)
Al1 Er2 Er1 6_567 1_556 55.61(6)
Al2 Er2 Er1 5_666 1_556 104.38(10)
Al2 Er2 Er1 5_566 1_556 104.38(10)
Ge1 Er2 Er1 2 1_556 99.52(4)
Er1 Er2 Er1 . 1_556 150.05(4)
Ni2 Er2 Er3 1_556 . 76.27(7)
Ge2 Er2 Er3 6_566 . 52.50(3)
Ge2 Er2 Er3 6_666 . 52.50(3)
Ge1 Er2 Er3 6_567 . 135.05(2)
Ge1 Er2 Er3 6_667 . 135.05(2)
Ni1 Er2 Er3 6_566 . 98.31(6)
Ni1 Er2 Er3 6_666 . 98.31(6)
Ni1 Er2 Er3 2_556 . 156.38(6)
Al1 Er2 Er3 6_667 . 104.36(7)
Al1 Er2 Er3 6_567 . 104.36(7)
Al2 Er2 Er3 5_666 . 55.39(9)
Al2 Er2 Er3 5_566 . 55.39(9)
Ge1 Er2 Er3 2 . 109.29(4)
Er1 Er2 Er3 . . 58.76(2)
Er1 Er2 Er3 1_556 . 151.19(3)
Ni2 Er3 Ge2 . 5_666 102.77(4)
Ni2 Er3 Ge2 . 6_566 102.77(4)
Ge2 Er3 Ge2 5_666 6_566 154.46(7)
Ni2 Er3 Ge2 . 6_666 102.77(4)
Ge2 Er3 Ge2 5_666 6_666 84.57(5)
Ge2 Er3 Ge2 6_566 6_666 89.82(5)
Ni2 Er3 Ge2 . 5_566 102.77(4)
Ge2 Er3 Ge2 5_666 5_566 89.82(5)
Ge2 Er3 Ge2 6_566 5_566 84.57(5)
Ge2 Er3 Ge2 6_666 5_566 154.46(7)
Ni2 Er3 Al2 . 5_666 139.48(7)
Ge2 Er3 Al2 5_666 5_666 51.19(5)
Ge2 Er3 Al2 6_566 5_666 106.90(6)
Ge2 Er3 Al2 6_666 5_666 51.19(5)
Ge2 Er3 Al2 5_566 5_666 106.90(6)
Ni2 Er3 Al2 . 5_566 139.48(7)
Ge2 Er3 Al2 5_666 5_566 106.90(6)
Ge2 Er3 Al2 6_566 5_566 51.19(5)
Ge2 Er3 Al2 6_666 5_566 106.90(6)
Ge2 Er3 Al2 5_566 5_566 51.19(5)
Al2 Er3 Al2 5_666 5_566 81.04(14)
Ni2 Er3 Al1 . 6_566 50.40(6)
Ge2 Er3 Al1 5_666 6_566 151.66(9)
Ge2 Er3 Al1 6_566 6_566 53.25(7)
Ge2 Er3 Al1 6_666 6_566 108.12(6)
Ge2 Er3 Al1 5_566 6_566 88.32(5)
Al2 Er3 Al1 5_666 6_566 154.56(7)
Al2 Er3 Al1 5_566 6_566 93.79(8)
Ni2 Er3 Al1 . 5_566 50.40(6)
Ge2 Er3 Al1 5_666 5_566 108.12(6)
Ge2 Er3 Al1 6_566 5_566 88.32(5)
Ge2 Er3 Al1 6_666 5_566 151.66(8)
Ge2 Er3 Al1 5_566 5_566 53.25(7)
Al2 Er3 Al1 5_666 5_566 154.56(7)
Al2 Er3 Al1 5_566 5_566 93.79(8)
Al1 Er3 Al1 6_566 5_566 50.04(14)
Ni2 Er3 Al1 . 6_666 50.40(6)
Ge2 Er3 Al1 5_666 6_666 88.32(5)
Ge2 Er3 Al1 6_566 6_666 108.12(6)
Ge2 Er3 Al1 6_666 6_666 53.25(7)
Ge2 Er3 Al1 5_566 6_666 151.66(8)
Al2 Er3 Al1 5_666 6_666 93.79(8)
Al2 Er3 Al1 5_566 6_666 154.56(7)
Al1 Er3 Al1 6_566 6_666 80.19(9)
Al1 Er3 Al1 5_566 6_666 100.79(13)
Ni2 Er3 Al1 . 5_666 50.40(6)
Ge2 Er3 Al1 5_666 5_666 53.25(7)
Ge2 Er3 Al1 6_566 5_666 151.66(8)
Ge2 Er3 Al1 6_666 5_666 88.32(5)
Ge2 Er3 Al1 5_566 5_666 108.12(6)
Al2 Er3 Al1 5_666 5_666 93.79(8)
Al2 Er3 Al1 5_566 5_666 154.56(7)
Al1 Er3 Al1 6_566 5_666 100.79(13)
Al1 Er3 Al1 5_566 5_666 80.19(9)
Al1 Er3 Al1 6_666 5_666 50.04(14)
Ni2 Er3 Er1 . . 76.88(2)
Ge2 Er3 Er1 5_666 . 134.86(2)
Ge2 Er3 Er1 6_566 . 52.76(3)
Ge2 Er3 Er1 6_666 . 52.76(3)
Ge2 Er3 Er1 5_566 . 134.86(2)
Al2 Er3 Er1 5_666 . 99.933(18)
Al2 Er3 Er1 5_566 . 99.933(19)
Al1 Er3 Er1 6_566 . 56.18(6)
Al1 Er3 Er1 5_566 . 105.50(8)
Al1 Er3 Er1 6_666 . 56.18(6)
Al1 Er3 Er1 5_666 . 105.50(8)
Ni2 Er3 Er1 . 2_565 76.88(2)
Ge2 Er3 Er1 5_666 2_565 52.76(3)
Ge2 Er3 Er1 6_566 2_565 134.86(2)
Ge2 Er3 Er1 6_666 2_565 134.86(2)
Ge2 Er3 Er1 5_566 2_565 52.76(3)
Al2 Er3 Er1 5_666 2_565 99.933(19)
Al2 Er3 Er1 5_566 2_565 99.933(19)
Al1 Er3 Er1 6_566 2_565 105.50(8)
Al1 Er3 Er1 5_566 2_565 56.18(6)
Al1 Er3 Er1 6_666 2_565 105.50(8)
Al1 Er3 Er1 5_666 2_565 56.18(6)
Er1 Er3 Er1 . 2_565 153.77(4)
Ni2 Er3 Er2 . 2_565 136.301(18)
Ge2 Er3 Er2 5_666 2_565 51.34(3)
Ge2 Er3 Er2 6_566 2_565 107.76(4)
Ge2 Er3 Er2 6_666 2_565 107.76(4)
Ge2 Er3 Er2 5_566 2_565 51.34(3)
Al2 Er3 Er2 5_666 2_565 56.66(4)
Al2 Er3 Er2 5_566 2_565 56.66(4)
Al1 Er3 Er2 6_566 2_565 138.85(5)
Al1 Er3 Er2 5_566 2_565 99.71(7)
Al1 Er3 Er2 6_666 2_565 138.85(5)
Al1 Er3 Er2 5_666 2_565 99.71(7)
Er1 Er3 Er2 . 2_565 146.81(4)
Er1 Er3 Er2 2_565 2_565 59.417(19)
Ni2 Er3 Er2 . . 136.301(18)
Ge2 Er3 Er2 5_666 . 107.76(4)
Ge2 Er3 Er2 6_566 . 51.34(3)
Ge2 Er3 Er2 6_666 . 51.34(3)
Ge2 Er3 Er2 5_566 . 107.76(4)
Al2 Er3 Er2 5_666 . 56.66(4)
Al2 Er3 Er2 5_566 . 56.66(4)
Al1 Er3 Er2 6_566 . 99.71(7)
Al1 Er3 Er2 5_566 . 138.85(5)
Al1 Er3 Er2 6_666 . 99.71(7)
Al1 Er3 Er2 5_666 . 138.85(5)
Er1 Er3 Er2 . . 59.417(19)
Er1 Er3 Er2 2_565 . 146.81(4)
Er2 Er3 Er2 2_565 . 87.40(4)
Ni1 Ge1 Ni1 5_556 5_656 117.61(14)
Ni1 Ge1 Ni1 5_556 1_556 81.18(9)
Ni1 Ge1 Ni1 5_656 1_556 81.18(9)
Ni1 Ge1 Al1 5_556 . 121.10(7)
Ni1 Ge1 Al1 5_656 . 121.10(7)
Ni1 Ge1 Al1 1_556 . 111.51(12)
Ni1 Ge1 Er1 5_556 2 73.00(7)
Ni1 Ge1 Er1 5_656 2 73.00(7)
Ni1 Ge1 Er1 1_556 2 128.41(9)
Al1 Ge1 Er1 . 2 120.08(10)
Ni1 Ge1 Er2 5_556 6_657 144.86(9)
Ni1 Ge1 Er2 5_656 6_657 67.15(7)
Ni1 Ge1 Er2 1_556 6_657 64.73(5)
Al1 Ge1 Er2 . 6_657 68.26(7)
Er1 Ge1 Er2 2 6_657 135.15(2)
Ni1 Ge1 Er2 5_556 6_557 67.15(7)
Ni1 Ge1 Er2 5_656 6_557 144.86(9)
Ni1 Ge1 Er2 1_556 6_557 64.73(5)
Al1 Ge1 Er2 . 6_557 68.26(7)
Er1 Ge1 Er2 2 6_557 135.15(2)
Er2 Ge1 Er2 6_657 6_557 89.66(5)
Ni1 Ge1 Er1 5_556 6_556 65.15(6)
Ni1 Ge1 Er1 5_656 6_556 141.00(9)
Ni1 Ge1 Er1 1_556 6_556 134.40(3)
Al1 Ge1 Er1 . 6_556 67.03(6)
Er1 Ge1 Er1 2 6_556 71.22(4)
Er2 Ge1 Er1 6_657 6_556 135.29(7)
Er2 Ge1 Er1 6_557 6_556 73.96(3)
Ni1 Ge1 Er1 5_556 6_656 141.00(9)
Ni1 Ge1 Er1 5_656 6_656 65.15(6)
Ni1 Ge1 Er1 1_556 6_656 134.40(3)
Al1 Ge1 Er1 . 6_656 67.03(6)
Er1 Ge1 Er1 2 6_656 71.22(4)
Er2 Ge1 Er1 6_657 6_656 73.96(3)
Er2 Ge1 Er1 6_557 6_656 135.29(7)
Er1 Ge1 Er1 6_556 6_656 88.84(5)
Ni1 Ge1 Er2 5_556 2 59.65(7)
Ni1 Ge1 Er2 5_656 2 59.65(7)
Ni1 Ge1 Er2 1_556 2 60.05(7)
Al1 Ge1 Er2 . 2 171.56(10)
Er1 Ge1 Er2 2 2 68.36(4)
Er2 Ge1 Er2 6_657 2 106.11(5)
Er2 Ge1 Er2 6_557 2 106.11(5)
Er1 Ge1 Er2 6_556 2 118.29(4)
Er1 Ge1 Er2 6_656 2 118.29(4)
Ni1 Ge2 Al2 . . 117.94(13)
Ni1 Ge2 Al1 . . 122.91(12)
Al2 Ge2 Al1 . . 119.15(15)
Ni1 Ge2 Er2 . 6_556 66.64(5)
Al2 Ge2 Er2 . 6_556 71.31(7)
Al1 Ge2 Er2 . 6_556 134.14(3)
Ni1 Ge2 Er2 . 6_656 66.64(5)
Al2 Ge2 Er2 . 6_656 71.31(7)
Al1 Ge2 Er2 . 6_656 134.14(3)
Er2 Ge2 Er2 6_556 6_656 91.66(5)
Ni1 Ge2 Er1 . 6_656 73.18(6)
Al2 Ge2 Er1 . 6_656 134.18(3)
Al1 Ge2 Er1 . 6_656 67.90(6)
Er2 Ge2 Er1 6_556 6_656 139.72(6)
Er2 Ge2 Er1 6_656 6_656 74.68(2)
Ni1 Ge2 Er1 . 6_556 73.18(6)
Al2 Ge2 Er1 . 6_556 134.18(3)
Al1 Ge2 Er1 . 6_556 67.90(6)
Er2 Ge2 Er1 6_556 6_556 74.68(2)
Er2 Ge2 Er1 6_656 6_556 139.72(6)
Er1 Ge2 Er1 6_656 6_556 91.43(5)
Ni1 Ge2 Er3 . 5_666 135.06(2)
Al2 Ge2 Er3 . 5_666 69.36(7)
Al1 Ge2 Er3 . 5_666 68.61(7)
Er2 Ge2 Er3 6_556 5_666 140.67(6)
Er2 Ge2 Er3 6_656 5_666 76.15(3)
Er1 Ge2 Er3 6_656 5_666 73.40(3)
Er1 Ge2 Er3 6_556 5_666 136.49(6)
Ni1 Ge2 Er3 . 5_566 135.06(2)
Al2 Ge2 Er3 . 5_566 69.36(7)
Al1 Ge2 Er3 . 5_566 68.61(7)
Er2 Ge2 Er3 6_556 5_566 76.15(3)
Er2 Ge2 Er3 6_656 5_566 140.67(6)
Er1 Ge2 Er3 6_656 5_566 136.49(6)
Er1 Ge2 Er3 6_556 5_566 73.40(3)
Er3 Ge2 Er3 5_666 5_566 89.82(5)
Ge1 Ni1 Ge1 5_556 5_656 117.61(14)
Ge1 Ni1 Ge2 5_556 . 116.12(7)
Ge1 Ni1 Ge2 5_656 . 116.12(7)
Ge1 Ni1 Ge1 5_556 1_554 98.82(9)
Ge1 Ni1 Ge1 5_656 1_554 98.82(9)
Ge2 Ni1 Ge1 . 1_554 104.55(11)
Ge1 Ni1 Er1 5_556 2 66.32(7)
Ge1 Ni1 Er1 5_656 2 66.32(7)
Ge2 Ni1 Er1 . 2 109.07(10)
Ge1 Ni1 Er1 1_554 2 146.38(12)
Ge1 Ni1 Er2 5_556 6_656 161.21(11)
Ge1 Ni1 Er2 5_656 6_656 75.21(5)
Ge2 Ni1 Er2 . 6_656 64.06(6)
Ge1 Ni1 Er2 1_554 6_656 64.32(6)
Er1 Ni1 Er2 2 6_656 132.33(5)
Ge1 Ni1 Er2 5_556 6_556 75.21(5)
Ge1 Ni1 Er2 5_656 6_556 161.21(11)
Ge2 Ni1 Er2 . 6_556 64.06(6)
Ge1 Ni1 Er2 1_554 6_556 64.32(6)
Er1 Ni1 Er2 2 6_556 132.33(5)
Er2 Ni1 Er2 6_656 6_556 89.27(7)
Ge1 Ni1 Er2 5_556 2_554 64.69(7)
Ge1 Ni1 Er2 5_656 2_554 64.69(7)
Ge2 Ni1 Er2 . 2_554 177.41(11)
Ge1 Ni1 Er2 1_554 2_554 72.86(8)
Er1 Ni1 Er2 2 2_554 73.52(7)
Er2 Ni1 Er2 6_656 2_554 114.30(7)
Er2 Ni1 Er2 6_556 2_554 114.30(7)
Ge1 Ni1 Er1 5_556 6_656 128.12(10)
Ge1 Ni1 Er1 5_656 6_656 60.59(5)
Ge2 Ni1 Er1 . 6_656 60.03(6)
Ge1 Ni1 Er1 1_554 6_656 133.01(6)
Er1 Ni1 Er1 2 6_656 67.65(5)
Er2 Ni1 Er1 6_656 6_656 69.45(4)
Er2 Ni1 Er1 6_556 6_656 124.02(9)
Er2 Ni1 Er1 2_554 6_656 121.67(7)
Ge1 Ni1 Er1 5_556 6_556 60.59(5)
Ge1 Ni1 Er1 5_656 6_556 128.12(10)
Ge2 Ni1 Er1 . 6_556 60.03(6)
Ge1 Ni1 Er1 1_554 6_556 133.01(6)
Er1 Ni1 Er1 2 6_556 67.65(5)
Er2 Ni1 Er1 6_656 6_556 124.02(9)
Er2 Ni1 Er1 6_556 6_556 69.45(4)
Er2 Ni1 Er1 2_554 6_556 121.67(7)
Er1 Ni1 Er1 6_656 6_556 80.77(6)
Al1 Ni2 Al1 5_666 6_566 146.8(2)
Al1 Ni2 Al1 5_666 6_666 63.47(15)
Al1 Ni2 Al1 6_566 6_666 106.47(16)
Al1 Ni2 Al1 5_666 5_566 106.47(16)
Al1 Ni2 Al1 6_566 5_566 63.47(15)
Al1 Ni2 Al1 6_666 5_566 146.8(2)
Al1 Ni2 Al2 5_666 5_565 143.94(12)
Al1 Ni2 Al2 6_566 5_565 62.69(12)
Al1 Ni2 Al2 6_666 5_565 143.94(12)
Al1 Ni2 Al2 5_566 5_565 62.69(12)
Al1 Ni2 Al2 5_666 5_665 62.69(12)
Al1 Ni2 Al2 6_566 5_665 143.94(12)
Al1 Ni2 Al2 6_666 5_665 62.69(12)
Al1 Ni2 Al2 5_566 5_665 143.94(12)
Al2 Ni2 Al2 5_565 5_665 104.5(2)
Al1 Ni2 Er3 5_666 . 73.40(12)
Al1 Ni2 Er3 6_566 . 73.40(12)
Al1 Ni2 Er3 6_666 . 73.40(12)
Al1 Ni2 Er3 5_566 . 73.40(12)
Al2 Ni2 Er3 5_565 . 127.73(12)
Al2 Ni2 Er3 5_665 . 127.73(12)
Al1 Ni2 Er2 5_666 1_554 126.75(8)
Al1 Ni2 Er2 6_566 1_554 71.76(8)
Al1 Ni2 Er2 6_666 1_554 71.76(8)
Al1 Ni2 Er2 5_566 1_554 126.75(8)
Al2 Ni2 Er2 5_565 1_554 72.20(7)
Al2 Ni2 Er2 5_665 1_554 72.20(7)
Er3 Ni2 Er2 . 1_554 119.97(7)
Al1 Ni2 Er2 5_666 2_564 71.76(8)
Al1 Ni2 Er2 6_566 2_564 126.75(8)
Al1 Ni2 Er2 6_666 2_564 126.75(8)
Al1 Ni2 Er2 5_566 2_564 71.76(8)
Al2 Ni2 Er2 5_565 2_564 72.20(7)
Al2 Ni2 Er2 5_665 2_564 72.20(7)
Er3 Ni2 Er2 . 2_564 119.97(7)
Er2 Ni2 Er2 1_554 2_564 120.06(13)
Ni2 Al1 Ni2 5_666 5_566 106.47(16)
Ni2 Al1 Al2 5_666 1_556 59.26(11)
Ni2 Al1 Al2 5_566 1_556 59.26(11)
Ni2 Al1 Al1 5_666 2 58.26(8)
Ni2 Al1 Al1 5_566 2 58.26(8)
Al2 Al1 Al1 1_556 2 59.84(10)
Ni2 Al1 Ge1 5_666 . 115.29(10)
Ni2 Al1 Ge1 5_566 . 115.29(10)
Al2 Al1 Ge1 1_556 . 104.19(15)
Al1 Al1 Ge1 2 . 164.03(9)
Ni2 Al1 Ge2 5_666 . 113.28(13)
Ni2 Al1 Ge2 5_566 . 113.28(13)
Al2 Al1 Ge2 1_556 . 162.66(18)
Al1 Al1 Ge2 2 . 102.81(9)
Ge1 Al1 Ge2 . . 93.15(14)
Ni2 Al1 Er1 5_666 6_556 167.47(13)
Ni2 Al1 Er1 5_566 6_556 85.82(4)
Al2 Al1 Er1 1_556 6_556 131.84(9)
Al1 Al1 Er1 2 6_556 129.97(6)
Ge1 Al1 Er1 . 6_556 59.47(7)
Ge2 Al1 Er1 . 6_556 57.94(7)
Ni2 Al1 Er1 5_666 6_656 85.82(4)
Ni2 Al1 Er1 5_566 6_656 167.47(13)
Al2 Al1 Er1 1_556 6_656 131.84(9)
Al1 Al1 Er1 2 6_656 129.97(6)
Ge1 Al1 Er1 . 6_656 59.47(7)
Ge2 Al1 Er1 . 6_656 57.94(7)
Er1 Al1 Er1 6_556 6_656 81.81(10)
Ni2 Al1 Er2 5_666 6_657 58.15(7)
Ni2 Al1 Er2 5_566 6_657 120.59(16)
Al2 Al1 Er2 1_556 6_657 65.80(9)
Al1 Al1 Er2 2 6_657 110.48(7)
Ge1 Al1 Er2 . 6_657 58.48(7)
Ge2 Al1 Er2 . 6_657 125.66(10)
Er1 Al1 Er2 6_556 6_657 117.95(12)
Er1 Al1 Er2 6_656 6_657 67.75(5)
Ni2 Al1 Er2 5_666 6_557 120.59(16)
Ni2 Al1 Er2 5_566 6_557 58.15(7)
Al2 Al1 Er2 1_556 6_557 65.80(9)
Al1 Al1 Er2 2 6_557 110.48(7)
Ge1 Al1 Er2 . 6_557 58.48(7)
Ge2 Al1 Er2 . 6_557 125.66(10)
Er1 Al1 Er2 6_556 6_557 67.75(5)
Er1 Al1 Er2 6_656 6_557 117.95(12)
Er2 Al1 Er2 6_657 6_557 80.63(9)
Ni2 Al1 Er3 5_666 5_566 118.40(14)
Ni2 Al1 Er3 5_566 5_566 56.20(9)
Al2 Al1 Er3 1_556 5_566 109.80(11)
Al1 Al1 Er3 2 5_566 64.98(7)
Ge1 Al1 Er3 . 5_566 125.59(10)
Ge2 Al1 Er3 . 5_566 58.14(7)
Er1 Al1 Er3 6_556 5_566 66.17(5)
Er1 Al1 Er3 6_656 5_566 116.07(12)
Er2 Al1 Er3 6_657 5_566 175.23(14)
Er2 Al1 Er3 6_557 5_566 99.390(19)
Ni2 Al1 Er3 5_666 5_666 56.20(9)
Ni2 Al1 Er3 5_566 5_666 118.40(14)
Al2 Al1 Er3 1_556 5_666 109.80(11)
Al1 Al1 Er3 2 5_666 64.98(7)
Ge1 Al1 Er3 . 5_666 125.59(10)
Ge2 Al1 Er3 . 5_666 58.14(7)
Er1 Al1 Er3 6_556 5_666 116.07(12)
Er1 Al1 Er3 6_656 5_666 66.17(5)
Er2 Al1 Er3 6_657 5_666 99.390(19)
Er2 Al1 Er3 6_557 5_666 175.23(14)
Er3 Al1 Er3 5_566 5_666 80.19(9)
Ni2 Al2 Ni2 5_565 5_665 104.5(2)
Ni2 Al2 Ge2 5_565 2 114.15(4)
Ni2 Al2 Ge2 5_665 2 114.15(4)
Ni2 Al2 Ge2 5_565 . 114.15(4)
Ni2 Al2 Ge2 5_665 . 114.15(4)
Ge2 Al2 Ge2 2 . 96.1(2)
Ni2 Al2 Al1 5_565 1_554 58.05(12)
Ni2 Al2 Al1 5_665 1_554 58.05(12)
Ge2 Al2 Al1 2 1_554 162.12(19)
Ge2 Al2 Al1 . 1_554 101.81(9)
Ni2 Al2 Al1 5_565 2_554 58.05(12)
Ni2 Al2 Al1 5_665 2_554 58.05(12)
Ge2 Al2 Al1 2 2_554 101.81(9)
Ge2 Al2 Al1 . 2_554 162.12(19)
Al1 Al2 Al1 1_554 2_554 60.3(2)
Ni2 Al2 Er3 5_565 5_666 168.25(18)
Ni2 Al2 Er3 5_665 5_666 87.21(7)
Ge2 Al2 Er3 2 5_666 59.45(10)
Ge2 Al2 Er3 . 5_666 59.45(10)
Al1 Al2 Er3 1_554 5_666 131.09(5)
Al1 Al2 Er3 2_554 5_666 131.09(5)
Ni2 Al2 Er3 5_565 5_566 87.21(7)
Ni2 Al2 Er3 5_665 5_566 168.25(18)
Ge2 Al2 Er3 2 5_566 59.45(10)
Ge2 Al2 Er3 . 5_566 59.45(10)
Al1 Al2 Er3 1_554 5_566 131.09(5)
Al1 Al2 Er3 2_554 5_566 131.09(5)
Er3 Al2 Er3 5_666 5_566 81.04(14)
Ni2 Al2 Er2 5_565 5_666 118.27(13)
Ni2 Al2 Er2 5_665 5_666 57.40(4)
Ge2 Al2 Er2 2 5_666 57.70(3)
Ge2 Al2 Er2 . 5_666 127.27(14)
Al1 Al2 Er2 1_554 5_666 109.82(16)
Al1 Al2 Er2 2_554 5_666 64.47(8)
Er3 Al2 Er2 5_666 5_666 67.95(5)
Er3 Al2 Er2 5_566 5_666 117.15(12)
Ni2 Al2 Er2 5_565 6_556 57.40(4)
Ni2 Al2 Er2 5_665 6_556 118.27(13)
Ge2 Al2 Er2 2 6_556 127.27(14)
Ge2 Al2 Er2 . 6_556 57.70(3)
Al1 Al2 Er2 1_554 6_556 64.46(8)
Al1 Al2 Er2 2_554 6_556 109.82(16)
Er3 Al2 Er2 5_666 6_556 117.15(12)
Er3 Al2 Er2 5_566 6_556 67.95(5)
Er2 Al2 Er2 5_666 6_556 173.9(2)
Ni2 Al2 Er2 5_565 5_566 57.40(4)
Ni2 Al2 Er2 5_665 5_566 118.27(13)
Ge2 Al2 Er2 2 5_566 57.70(3)
Ge2 Al2 Er2 . 5_566 127.27(14)
Al1 Al2 Er2 1_554 5_566 109.82(16)
Al1 Al2 Er2 2_554 5_566 64.47(8)
Er3 Al2 Er2 5_666 5_566 117.15(12)
Er3 Al2 Er2 5_566 5_566 67.95(5)
Er2 Al2 Er2 5_666 5_566 79.59(2)
Er2 Al2 Er2 6_556 5_566 100.08(3)
Ni2 Al2 Er2 5_565 6_656 118.27(13)
Ni2 Al2 Er2 5_665 6_656 57.40(4)
Ge2 Al2 Er2 2 6_656 127.27(14)
Ge2 Al2 Er2 . 6_656 57.70(3)
Al1 Al2 Er2 1_554 6_656 64.47(8)
Al1 Al2 Er2 2_554 6_656 109.82(16)
Er3 Al2 Er2 5_666 6_656 67.95(5)
Er3 Al2 Er2 5_566 6_656 117.15(12)
Er2 Al2 Er2 5_666 6_656 100.08(3)
Er2 Al2 Er2 6_556 6_656 79.59(2)
Er2 Al2 Er2 5_566 6_656 173.9(2)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Er1 Ge2 6_666 2.9027(13) y
Er1 Ge2 6_566 2.9027(13) ?
Er1 Ge1 2 2.9215(18) y
Er1 Ni1 2 2.942(3) y
Er1 Ge1 6_566 2.9690(14) y
Er1 Ge1 6_666 2.9690(14) ?
Er1 Al1 6_666 3.173(3) y
Er1 Al1 6_566 3.173(3) ?
Er1 Ni1 6_666 3.207(2) y
Er1 Ni1 6_566 3.207(2) ?
Er1 Er1 5_566 3.4299(15) y
Er1 Er1 5_666 3.4299(15) ?
Er1 Er3 . 3.4940(9) y
Er1 Er2 . 3.5180(10) y
Er1 Er2 1_554 3.5593(10) y
Er2 Ni2 1_556 2.873(2) y
Er2 Ge2 6_566 2.8971(12) y
Er2 Ge2 6_666 2.8971(13) ?
Er2 Ge1 6_567 2.9475(13) y
Er2 Ge1 6_667 2.9475(13) ?
Er2 Ni1 6_566 2.9576(19) y
Er2 Ni1 6_666 2.9576(19) ?
Er2 Ni1 2_556 3.005(3) y
Er2 Al1 6_667 3.212(3) y
Er2 Al1 6_567 3.212(3) ?
Er2 Al2 5_666 3.2467(8) y
Er2 Al2 5_566 3.2467(8) ?
Er2 Ge1 2 3.314(2) y
Er2 Er1 1_556 3.5593(10) ?
Er2 Er3 . 3.6020(12) y
Er3 Ni2 . 2.798(4) y
Er3 Ge2 5_666 2.9433(12) y
Er3 Ge2 6_566 2.9433(12) ?
Er3 Ge2 6_666 2.9433(12) ?
Er3 Ge2 5_566 2.9433(12) ?
Er3 Al2 5_666 3.198(5) y
Er3 Al2 5_566 3.198(5) ?
Er3 Al1 6_566 3.227(3) y
Er3 Al1 5_566 3.227(3) ?
Er3 Al1 6_666 3.227(3) ?
Er3 Al1 5_666 3.227(3) ?
Er3 Er1 2_565 3.4940(9) ?
Er3 Er2 2_565 3.6020(12) ?
Ge1 Ni1 5_556 2.4293(18) y
Ge1 Ni1 5_656 2.4293(18) ?
Ge1 Ni1 1_556 2.540(3) y
Ge1 Al1 . 2.771(4) y
Ge1 Er1 2 2.9215(18) ?
Ge1 Er2 6_657 2.9475(13) ?
Ge1 Er2 6_557 2.9475(13) ?
Ge1 Er1 6_556 2.9690(14) ?
Ge1 Er1 6_656 2.9690(14) ?
Ge1 Er2 2 3.314(2) ?
Ge2 Ni1 . 2.442(3) y
Ge2 Al2 . 2.663(4) y
Ge2 Al1 . 2.777(4) y
Ge2 Er2 6_556 2.8971(12) ?
Ge2 Er2 6_656 2.8971(12) ?
Ge2 Er1 6_656 2.9027(13) ?
Ge2 Er1 6_556 2.9027(13) ?
Ge2 Er3 5_666 2.9433(12) ?
Ge2 Er3 5_566 2.9433(12) ?
Ni1 Ge1 5_556 2.4293(18) ?
Ni1 Ge1 5_656 2.4293(18) ?
Ni1 Ge1 1_554 2.540(3) ?
Ni1 Er1 2 2.942(3) ?
Ni1 Er2 6_656 2.9576(19) ?
Ni1 Er2 6_556 2.9576(19) ?
Ni1 Er2 2_554 3.005(3) ?
Ni1 Er1 6_656 3.207(2) ?
Ni1 Er1 6_556 3.207(2) ?
Ni2 Al1 5_666 2.594(3) y
Ni2 Al1 6_566 2.594(3) ?
Ni2 Al1 6_666 2.594(3) ?
Ni2 Al1 5_566 2.594(3) ?
Ni2 Al2 5_565 2.627(4) y
Ni2 Al2 5_665 2.627(4) ?
Ni2 Er2 1_554 2.873(2) ?
Ni2 Er2 2_564 2.873(2) ?
Al1 Ni2 5_666 2.594(3) ?
Al1 Ni2 5_566 2.594(3) ?
Al1 Al2 1_556 2.716(6) y
Al1 Al1 2 2.729(8) y
Al1 Er1 6_556 3.173(3) ?
Al1 Er1 6_656 3.173(3) ?
Al1 Er2 6_657 3.212(3) ?
Al1 Er2 6_557 3.212(3) ?
Al1 Er3 5_566 3.227(3) ?
Al1 Er3 5_666 3.227(3) ?
Al2 Ni2 5_565 2.627(4) ?
Al2 Ni2 5_665 2.627(4) ?
Al2 Ge2 2 2.663(4) ?
Al2 Al1 1_554 2.716(6) ?
Al2 Al1 2_554 2.716(6) ?
Al2 Er3 5_666 3.198(5) ?
Al2 Er3 5_566 3.198(5) ?
Al2 Er2 5_666 3.2467(8) ?
Al2 Er2 6_556 3.2467(8) ?
Al2 Er2 5_566 3.2467(8) ?
Al2 Er2 6_656 3.2467(8) ?
